Abstract
Quantum spin1/2 kagome Heisenberg antiferromagnet is the representative frustrated system possibly hosting a spin liquid. Clarifying the nature of this elusive topological phase is a key challenge in condensed matter; however, even identifying it still remains unsettled. Here we apply a magnetic field and discover a series of spingapped phases appearing at five different fractions of magnetization by means of a grand canonical density matrix renormalization group, an unbiased stateoftheart numerical technique. The magnetic field dopes magnons and first gives rise to a possible Z_{3} spin liquid plateau at 1/9 magnetization. Higher field induces a selforganized superlattice unit, a sixmembered ring of quantum spins, resembling an atomic orbital structure. Putting magnons into this unit one by one yields three quantum solid plateaus. We thus find that the magnetic field could control the transition between various emergent phases by continuously releasing the frustration.
Introduction
It is widely accepted that condensed matter orders at low temperatures by spontaneously breaking some sort of symmetry—translational symmetry in crystalline solids, time reversal and rotational symmetries in magnets, gauge symmetry in superconductors and so on. Whether they can escape from ordering and instead bear emergent states is a question that recurred over decades. A possible strategy to remove trivial orders is to design a model with fine balance of microscopic interactions, where the lowenergy states are frustrated and a macroscopic number of quasidegenerate states compete with each other. When quantum fluctuations between these states prevent a selection of particular order, one ends up with quantumdisordered spin liquids. Modern theories have brought us new insight by identifying spin liquids as topological phases of matter^{1,2}. Even if such topological phases are not formed, the resultant phase would also be nontrivial; its smallest disentangled unit could consist of several degrees of freedom—pairs of spins in spin ladders or valence bond solids and so on. Thus, characterizing the regime of such liquids and relevant nontrivial phases is now becoming an important challenge.
In reality, spin liquids are quite elusive^{3}. There are experimental studies on the several materials, suggesting the existence of a spin liquid, κ(BEDTTTF)_{2}Cu_{2}(CN)_{3} (ref. 4), BaCu_{3}V_{2}O_{8}(OH)_{2} (ref. 5) and ZnCu_{3}(OD)_{6}Cl_{2} (ref. 6). In theories, few candidates include a triangular lattice Mott insulator^{7} and spin1/2 kagome antiferromagnet^{8,9,10,11}, represented by the Hubbard and the Heisenberg models, respectively. However, theoretical information directly compared with the experimental data is still severely lacking.
Therefore, to find realistic theoretical models that could realize several nontrivial phases and could provide information relevant to experiments is essential. The phase transitions should better be controlled by the experimentally tunable parameter.
Here we show that quantum spin1/2 kagome Heisenberg antiferromagnet in an applied field could be an ideal playground, providing numbers of exotic quantum liquid and solid phases under field control. The model itself is already known as a representative frustrated system that embodies fine balance of interaction by the use of lattice geometry, and, more importantly, it is experimentally relevant. It is defined by the following Hamiltonian:
where S_{i} is a spin1/2 operator at the ith lattice site (S_{i}^{z} is the zcomponent), and J and H are the interaction coupling constant and the external magnetic field, respectively. The first summation denoted by runs over nearestneighbour pairs of sites of the kagome lattice of size N. The ground state at H=0 is possibly a spin liquid, but its detailed identification still suffers numerical difficulty.
A key numerical problem in quantum manybody models on twodimensional frustrated lattices is the lack of method that affords sizable results. The quantum MonteCarlo method suffers from the sign problem, and the exact diagonalization requires unbiased size scaling, which is unavailable at present. Regarding the kagome antiferromagnet, the multiscale entanglement renormalization supported a valence bond crystal ground state with a hexagonal unit cell of 36 spins^{11}, which was taken over by a Z_{2} gapped spin liquid lower in energy in the latest twodimensional density matrix renormalization group (DMRG) studies on a long cylinder^{8,9}. In addition, there is a recent study predicting a gapless U(1) liquid^{10}, and the issue remains unsettled.
Clarifying the nature of the model in an applied field also demands a severe numerical challenge; the magnetization process appears not as a curve but as a staircase of height ~1/N owing to finite size effect. Thus, what is known so far is the highly possible presence of a spingapped phase called plateau at a 1/3 magnetization^{12,13,14} and a jump of the magnetization from 7/9 to 1 at the saturation field^{15,16}. Whereas whether a 1/3 plateau is really a plateau^{12,13} or something else^{14} was not really concluded.
In the present article, we determine the bulk magnetization process of the kagome Heisenberg antiferromagnet by means of a grand canonical analysis^{17,18}. The system turns out to have five different plateau phases, and the magnetic field controls the successive phase transitions between these plateau phases and the gapless liquids in a strikingly analogous manner to the Hall conductivity of the quantum Hall effect^{19,20,21}. Two of the plateaus at the lower fields are the possible spin liquids, which are characterized by the finite topological dimensions. The latter three at the higher fields form a longrange order in a particular unit, a hexagonal plaquette consisting of a sixmembered ring of spins. This unit resembles a quantum mechanical atomic orbital that accommodates several magnons in its discrete energy levels. The magnetic field thus transforms the system from the highly frustrated liquid phases to the moderately frustrated solid ones.
Results
Magnetization curve
To overcome the numerical finite size effect, we apply the grand canonical DMRG, which was developed very recently^{17}, and was successfully applied to two dimensions^{18}. This method gives us a numerically exact and unbiased magnetization curve in the thermodynamic limit (see Methods). For example, if we choose the cylinder of a finite circumference and of length L, which is larger than ~10–20 lattice spacing, and perform a grand canonical analysis, we obtain a magnetization curve of an infinitely long cylinder of that fixed circumference (see Supplementary Fig. S1). As we need a result of a bulk system, equivalently spanned along three different directions of a kagome lattice, we choose a hexagonal cluster for the present calculation rather than a long cylinder.
Figure 1 shows the whole magnetization curve of the kagome antiferromagnet. Without ambiguity, one finds plateau structures at fractions, M/M_{sat}=0, 1/9, 1/3, 5/9 and 7/9, as well as a jump from the 7/9 plateau to the saturation value at exactly H_{sat}/J=3.0, where M_{sat} is the full magnetization. To verify the accuracy of our grand canonical curve, we perform a set of conventional DMRG calculation, both on a long cylinder with open ends (see Supplementary Fig. S1) and on an open hexagonal cluster. By comparing these results, we confirm that the grand canonical analysis successfully gives the magnetization curve within the typical accuracy of 10^{−3} (see Supplementary Note 1).
Singlet–triplet spin gap
The value of the singlet–triplet spin gap of the kagome antiferromagnet at zero field is still unsettled^{8,9,22}. The evaluated spin gaps after the size scaling in the three latest DMRG studies are not fully consistent; as for the cylindrical DMRG, ref. 9 has Δ=0.13(1) (the numerical data of refs 8 and 9 at various fixed circumferences are basically consistent). There, the size scaling is basically given first along the long leg of a cylinder and the extrapolation is given along the circumference of L≤20. As for ref. 22, they increased the size within N=36–108 by keeping the cluster to the squarelike shape with periodic boundaries and obtained Δ=0.055±0.005. In fact, we checked these results carefully with the similar scaling and found that the results depend much on the way the size scaling is performed^{23} (see Supplementary Notes 1 and 2).
By contrast, in our grand canonical calculation the size dependence becomes negligible (less than 10^{−3} in two dimensions, see Methods) once we enter a cluster size of the proper system length. Therefore, one could evaluate the spin gap by the onset value of H/J in the magnetization curve near zero field. In Fig. 1, we find Δ=0.05±0.02 (see the red shaded region), which is obtained on a hexagonal cluster.
We briefly mention that our results are fully consistent with the data of the previous conventional DMRG studies: in our grand canonical DMRG on a cylinder with fixed small circumference (see Supplementary Fig. S1), the spin gap gives more than twice as large values as the value mentioned above. This value should be compared with the data in ref. 9 on a long cylinder with the same circumference. For a proper extrapolation of the cylindrical results to a bulk twodimension, one needs to enlarge both the length and the circumferences simultaneously^{23}. In fact, our grand canonical spin gap on a hexagonal cluster is very close to those of ref. 22 on a square cluster.
Zero and 1/9 plateaus
The zero plateau ranging at 0≤H/J≤0.05 is the continuation of the zerofield ground state. Correspondingly, in our calculation the spin structure in real space turned out to be completely structureless (see Supplementary Fig. S2). One way to identify the nature of the spin liquid is to calculate the von Neumann entropy, S=−Tr(ρ ln ρ), defined on a subsystem of a long open cylinder by the conventional DMRG, where ρ is the reduced density matrix of the subsystem. The value should follow, S~η L_{y}−γ, where L_{y} is the circumference, η is a constant and γ=ln(D) is the topological entropy. In ref. 9, the topological dimension, D, of the ground state is given as D~2, which supports the gapped Z_{2} spin liquid.
In the 1/9plateau state, the real space profile of the spin structure is rather intriguing, several geometries breaking the translational symmetry are quasidegenerate (see Supplementary Fig. S2 and Supplementary Note 3), and their stability is sensitive to the shape and size of the cluster. We consider this to be the good reason that the symmetrybreaking long order is absent. Therefore, we perform the conventional DMRG and calculate the entanglement entropy of the 1/9plateau state in the same manner as refs 2 and 9, as shown in Fig. 2; to have the 1/9 magnetization, we need to keep the system size at the multiple of nine, and thus the choice of the clusters are limited compared with the calculation on the M/N=0 ground state. The topological dimension obtained in the L_{y}=0 limit seemingly gives the value D=3. Thus, the spingapped state at 1/9 magnetization is possibly a Z_{3} spin liquid, and is the first example of a spinliquid plateau induced by the magnetic field. Even a Z_{3} spin liquid itself has so far been observed only in a specified bosonic model^{24}, and the present model gives a more realistic setup. Further examination is required to identify the detailed nature of this phase.
Longrange ordered plateaus
In contrast to the first two plateaus, the rest of the plateaus have symmetrybreaking longrange orders. Figure 3a–c shows the real space profiles of the magnetization density for 1/3, 5/9 and 7/9 plateaus. All of them are based on a same unit of a hexagram, which holds nine lattice sites. This magnetic (extended) unit cell is three times as large as the original unit cell, namely, Q_{mag}=Q × 3=9, with the spin density shown in Fig. 3d. Such symmetrybreaking requires strong interaction between bosons, and the emergence of three such plateaus in a single system is already a quite unexpected matter to happen.
Discussion
In spin1/2 quantum magnets, a conventional (nontopological) nonmagnetic state basically comprises a singlet, a unit of spin 0, often represented by the quantum fluctuation between two spins, (↑↓–↓↑)/√2. A breaking of singlet yields a bosonic elementary particle carrying spin 1, which is called a magnon. The magnetic field controls the density of these bosons, serving as a chemical potential. As in the Mott insulator, there are particular values of the boson densities commensurate with the lattice periodicity^{25}, at which the gapped states are strongly pinned. At these fillings, a finite field range representing the spin gap is formed, which is the magnetization plateau.
It is known that the magnetization plateau emerges only when the quantity, Q_{mag} S(1−M/M_{sat}), is an integer^{26,27}, where Q_{mag} is the number of sites included in the unit period of the ground state and S is the spin quantum number, which is 1/2 for the present case.
With this in mind, let us discuss the nature of our plateaus. We first examine the magnetic structures of M/M_{sat}=0 and 1/9 plateaus, and find that they are possibly structureless in real space (see Supplementary Note 3). Namely, the period of the ground state is the same as that of the lattice unit cell, Q_{mag}=Q=3, which gives, Q_{mag} S(1−M/M_{sat})=3/2 and 4/3, respectively. As they are not integers but fractional numbers, the above conventional condition to have a plateau is not fulfilled. However, in two dimensions there is another way to form a spingapped state (plateau) other than the above mentioned interplay with the lattice; it is to form a structureless spin liquid. The elementary excitation of such spin liquids by the magnetic field is no longer a magnon, but a deconfined spinon, carrying spin 1/2. Although such exotic spinliquid plateaus could emerge at a fractional value of Q_{mag} S(1−M/M_{sat}), as discussed in field theoretical study^{28}, it had been observed neither in theoretical models nor in materials. In fact, the calculations on the entanglement entropy indicate that zeroth and the 1/9 plateau form the spinliquid phases of topological dimension D=2 and 3, respectively.
In contrast, in the latter three plateaus we find Q_{mag} S(1−M/M_{sat})=3, 2 and 1 (integers) for 1/3, 5/9 and 7/9 plateaus, respectively, all of which clearly fulfill the above conventional condition. Let us now discuss the origin of these solid plateaus.
In the 1/3 plateau, each triangular unit should hold a net magnetization of 1/2, which consists of one up spin 1/2 and two spins forming a singlet (see Fig. 4a). Similar to the zerofield Ising ground state, there are massive numbers of configuration of the 1/2magnetized triangular units^{29}, which is in fact a typical characteristic of the frustrated system. If these configurations are mixedup quantum mechanically, a liquid phase should emerge. To realize instead the solid state actually observed, one needs to select a particular configuration, and the problem reduces to how we pave this triangular unit on the kagome lattice to maximally gain energy.
In each configuration, one could draw a string along the singlet bonds of the triangular units as shown in the left panel of Fig. 4a. As every triangle shares its corners with the neighbouring triangles, the string never crosses with other strings, but continues until it meets itself again (otherwise it will extend toward infinity). In addition to the random configuration of strings, the representative two regular patterns are shown in Fig. 4a: a long string forming stripes and a shortest closed loop around the hexagon. One then needs to know which gains the energy, the longer string or the shorter loop, towing to the quantum mechanical resonance of spins along the string. The answer is the latter (see Supplementary Fig. S3a)—the kagome is fully tiled with hexagrams—a symmetrybreaking plaquette order is formed^{30}.
Once all the vertices of the hexagram (three sites/nine unit) are filled with a fully polarized upspin moment (S_{z}=1/2) at M/M_{sat}=1/3, a further simplified picture may work, focusing on each hexagonal plaquette and isolating it by effectively neglecting the quantum fluctuation between the plaquette and the vertices of the hexagram, as shown in Fig. 4b. This approximation is valid as far as the vertices of the hexagram are fully polarized. The interactions (J S^{z} S^{z}term) between the plaquette and vertices work as an internal magnetic field, H_{int}=−J per site on a plaquette. Figure 4c shows the magnetization process of the isolated plaquette in an effective field, H+H_{int}, namely the doping of magnons by the effective chemical potential. Each step of the big staircases corresponds to the increasing S_{z}value or the number of magnons in the isolated plaquette. Now, notice that the point where the upshift of the staircases crosses the bulk magnetization curve coincides with the inflection point of the curve. This indicates the following scenario: if we condense the massive numbers of hexagrams, the quantum fluctuations between them become coherent throughout the system and works to destroy the staircases from the edge toward the centre of the step. The curve above/below the inflection point is the ruin of the edge of upper/lower staircase. This result thus supports the picture that a hexagon works as a selforganized pseudo atomic orbital consisting of three discrete energy levels. Doping magnons to each level yields a series of plateaus starting from 1/3.
At present, the only other quantum magnet that possibly reveals comparably rich phase transitions is the SrCu_{2}(BO_{3})_{2} (refs 31, 32). However, the spingapped phases of this material are based on a conventional singlet. In forming solids, they expand the unit cell in several ways to allocate the singlets in a regular period in a sea of doped magnons. In contrast, in our kagome a single nontrivial unit based on a hexagram is selforganized by the quantum manybody effect. The doped magnons come into this cell in such a way that the electrons go into the quantum dots in an artificial semiconductor device.
The above picture then gives a strategy to design a system that could control the degree of frustration by the doping of particles; First, prepare an unfrustrated unit that could store several numbers of particles (in a kagome, this corresponds to a hexagon that could hold three magnons). Then connect them by the frustrated bonds. For example, this rule gives us a checkerboard lattice and its relevant pyroclore lattice. Their undoped ground states could be a spin liquid as far as the microscopic interactions are finely balanced. We predict that dopings will also give rise to interesting states of matter similar to the one we find in the kagome.
We further pay attention to the fact that the boseHubbard model at zero field^{33} and the projected quantum dimer model^{34}, both on the same kagome lattice, are considered to have Z_{2} liquids. Then, one may also expect the 5/9 and 7/9 plateaus to undergo a solidtospinliquid transition^{28} if the additional effect enhancing the quantum fluctuation is added to the Hamiltonian. The present findings will give some clue to find numbers of such exotic state of matter in kagome and in the above mentioned lattice models, many of which are still unexplored.
Regarding the laboratory systems of the kagome Heisenberg antiferromagnet, there are several candidates, for example, BaCu_{3}V_{2}O_{8}(OH)_{2} (ref. 5), ZnCu_{3}(OH)_{6}Cl_{2} (ref. 6), Cu_{3}V_{2}O_{7}(OH)_{2}·2H_{2}O (ref. 35) and Rb_{2}Cu_{3}SnF_{12} (ref. 36), whereas they are often distorted, anisotropic or include complicated interactions, and the establishing of the ideal kagome Heisenberg material is long awaited. Our bulk magnetization curve is the only data numerically obtained in lattice models that could be compared directly and quantitatively with experimental measurements. Such comparison could be used to identify them as an ideal kagome. Also, if a 1/9 plateau were to appear in the experimental magnetization curve, one could examine, by neutron measurements or some other local magnetic probelike nuclear magnetic resonance, whether the state is structureless in reality. The magneticspecific heat and thermal conductivity measurements could further give theorists a hint to know what kind of nonmagnetic and magnetic elementary excitations are possible for this newly emergent phase. Thus, our present findings would provide, both in theories and in experiments, a rich playground in search of open paradigms in quantum manybody physics.
Methods
Grand canonical analysis
The technique is developed very recently by the authors^{17,18}, and gives the infinitesimally small response to the change in the external field. The physical quantities we get mimic their thermodynamic limit within the order of 10^{−4} for one dimension and 10^{−3} for two dimensions, even in a relatively small cluster size of the order of N~10–100. We briefly summarize the essential framework; the method smoothly divides the finite size cluster into the centre part and the edges, and the main part reproduces the continuous bulk response by using the nearly zeroenergy edge state as a buffer. At a fixed system size and shape, we introduce the modulation of the energy scale by an externally given function, f( r), at a locationr, which smoothly deforms the Hamiltonian from the maximum at the centre of the system (r=0) to zero energy at the open cluster edges (r=R). After we obtain the proper eigen wave function of the deformed Hamiltonian, we evaluate the magnetization, . Now, remind that the total magnetization, , of the deformed Hamiltonian is a conserved quantity given by hand. However, the expectation value of the local magnetic density is no longer equal to M_{g}/N, but has a particular rdependence: it takes nearly a uniform value at the centre (though oscillating slightly, the mean values are uniform) and then often takes a peak or valley at the edges (see Suppplementary Fig. S4b and Suppplementary Note 5). This is because the system optimizes the wave function so as to realize the centre value, S^{z}(r~0), to its thermodynamic limit, M/N, at a given magnetic field. The excess/deficient magnetization, M_{g}−M, is absorbed/provided by the localized edge states of the cluster, which has the measure zero energy as f( r =R)~0. These edges serve as a grand canonical bath.
The cluster and the function used in the present calculation are given in Supplementary Fig. S4a. The numerical solver of the deformed Hamiltonian is not necessarily restricted to DMRG.
The reason why such mechanism works is discussed in detail in ref. 18 in the context of real space energy renormalization, together with applications to several twodimensional quantum spin systems and to the electronic systems.
Details of the DMRG calculation
We have used the DMRG^{37} as a solver of the deformed Hamiltonian of the ground canonical analysis. The accuracy of the results is systematically controlled by the number of basis states kept, m in the DMRG calculation and the typical error in the energy of the present calculations is around 10^{−4} for m=4,000. As discussed in the Results section, the aspect ratio closer to 1 gives the results closer to the bulk limit. Therefore, we adopt the hexagonal cluster of N=114 and 132, instead of a long cylinder. More details, including the numerical details of the results, are available in the Supplementary Fig. S4 and Supplementary Note 5.
Regarding the calculation on the entanglement entropy in Fig. 2, we used the conventional DMRG on a long cylinder with open edges and periodic circumferences. There, the number of states kept are m=2,000–10,000, and the data points displayed in Fig. 2a are derived after the extrapolation to 1/m=0.
Additional information
How to cite this article: Nishimoto, S. et al. Controlling frustrated liquids and solids with an applied field in a kagome Heisenberg antiferromagnet. Nat. Commun. 4:2287 doi: 10.1038/ncomms3287 (2013).
References
 1
Oshikawa, M. & Senthil, T. Fractionalization, topological order, and quasiparticle statistics. Phys. Rev. Lett. 96, 060601 (2006).
 2
Jiang, H.C., Wang, Z. & Balents, L. Identifying topological order by entanglement entropy. Nat. Phys. 8, 902–905 (2012).
 3
Balents, L. Spin liquids in frustrated magnets. Nature 464, 199–208 (2010).
 4
Shimizu, Y., Miyagawa, K., Kanoda, K., Maesato, M. & Saito, G. Spin liquid state in an organic Mott insulator with a triangular lattice. Phys. Rev. Lett. 91, 107001 (2003).
 5
Okamoto, Y., Yoshida, H. & Hiroi, Z. Vesignieite BaCu3V2O8(OH)2 as a candidate spin1/2 kagome antiferromagnet. J. Phys. Soc. Jpn 78, 033701 (2009).
 6
Han, T.H. et al. Fractionalized excitations in the spinliquid state of a kagomelattice antiferromagnet. Nature 492, 406–410 (2012).
 7
Morita, H., Watanabe, S. & Imada, M. Nonmagnetic insulating states near the Mott transitions on lattices with geometrical frustration and implications for κET2Cu2(CN)3 . J. Phys. Soc. Jpn 71, 2109–2112 (2002).
 8
Yan, S., Huse, D. A. & White, S. R. Spinliquid ground state of the S=1/2 kagome Heisenberg antiferromagnet. Science 332, 1173–1176 (2011).
 9
Depenbrock, S., McCulloch, I. P. & Schollwöck, U. Nature of the spinliquid ground state of the S=1/2 Heisenberg model on the kagome lattice. Phys. Rev. Lett. 109, 067201 (2012).
 10
Iqbal, Y., Becca, F., Sorella, S. & Poilblanc, D. Gapless spin liquid phase in spin1/2 Heisenberg antiferromagnet. Phys. Rev. B 87, 060405R (2013).
 11
Evenbly, G. & Vidal, G. Frustrated antiferromagnets with entanglement renormalization:ground state of the spin 1/2 Heisenberg model on a kagome lattice. Phys. Rev. Lett. 104, 187203 (2010).
 12
Hida, K. Magnetization process of the S=1 and 1/2 uniform and distorted kagome Heisenberg antiferromagnets. J. Phys. Soc. Jpn 70, 3673–3677 (2001).
 13
Honecker, A., Schulenburg, J. & Richter, J. Magnetization plateaus in frustrated antiferromagnetic quantum spin models. J. Phys. Condens. Matter 16, S749–S758 (2004).
 14
Nakano, H. & Sakai, T. Magnetization process of kagomelattice Heisenberg antiferromagnet. J. Phys. Soc. Jpn 79, 053707 (2010).
 15
Schulenburg, J., Honecker, A., Schnack, J., Richter, J. & Schmidt, H.J. Macroscopic magnetization jumps due to independent magnons in frustrated quantum spin lattices. Phys. Rev. Lett. 88, 167207 (2002).
 16
Zhitomirsky, M. E. & Tsunetsugu, H. Exact lowtemperature behavior of a kagome antiferromagnet at high fields. Phys. Rev. B 70, 100403(R) (2004).
 17
Hotta, C. & Shibata, N. Grand canonical finitesize numerical approaches: A route to measuring bulk properties in an applied field. Phys. Rev. B 86, 041108 (2012).
 18
Hotta, C., Nishimoto, S. & Shibata, N. Grand canonical finite size numerical approaches in one and two dimensions: real space energy renormalization and edge state generation. Phys. Rev. B 87, 115128 (2013).
 19
Tsui, D. C., Stormer, H. L. & Gossard, A. C. Twodimensional magnetotransport in the extreme quantum limit. Phys. Rev. Lett. 48, 1559–1562 (1982).
 20
Laughlin, R. B. Anomalous quantum hall effect: an incompressible quantum fluid with fractionally charged excitations. Phys. Rev. Lett. 50, 1395–1398 (1983).
 21
Klitzing, K., Dorda, G. & Pepper, M. New method for highaccuracy determination of the finestructure constant based on quantized hall resistance. Phys. Rev. Lett. 45, 494–497 (1980).
 22
Jiang, H. C., Weng, Z. Y. & Sheng, D. N. Density matrix renormalization group numerical study of the kagome antiferromagnet. Phys. Rev. Lett. 101, 117203 (2008).
 23
Sandvik, A. W. Finitesize scaling and boundary effects in twodimensional valencebond solids. Phys. Rev. B 85, 134407 (2012).
 24
Motrunich, O. I. Bosonic model with Z3 fractionalization. Phys. Rev. B 67, 115108 (2003).
 25
Fisher, M. P. A., Weichman, P. B., Grinstein, G. & Fisher, D. S. Boson localization and the superfluid–insulator transition. Phys. Rev. B 40, 546–570 (1989).
 26
Affleck, I. Spin gap and symmetry breaking in CuO2 layers and other antiferromagnets. Phys. Rev. B 37, 5186–5192 (1988).
 27
Oshikawa, M., Yamanaka, M. & Affleck, I. Magnetization plateaus in spin chains; “Haldane gap” for halfinteger spins. Phys. Rev. Lett. 78, 1984–1987 (1997).
 28
Tanaka, A., Totsuka, K. & Hu, X. Geometric phases and the magnetization process in quantum antiferromagnets. Phys. Rev. B 79, 064412 (2009).
 29
Moessner, R. & Sonhdi, S. L. Ising models of quantum frustration. Phys. Rev. B 63, 224401 (2001).
 30
Cabra, D. C. et al. Quantum kagome antiferromagnet in a magnetic field: Lowlying nonmagnetic excitations versus valencebond crystal order. Phys. Rev. B 71, 144420 (2005).
 31
Kageyama, H. et al. Exact dimer ground state and quantized magnetization plateaus in the twodimensional spin system, SrCu2 (BO3)2 . Phys. Rev. Lett. 82, 3168–3171 (1999).
 32
Miyahara, S. & Ueda, K. Exact dimer ground state of the two dimensional Heisenberg spin system SrCu2 (BO3)2 . Phys. Rev. Lett. 82, 3701–3704 (1999).
 33
Isakov, S. V., Melko, R. G. & Hastings, M. B. Topological entanglement entropy of a Bose–Hubbard spin liquid. Nat. Phys. 7, 772–775 (2011).
 34
Poilblanc, D., Mambrini, M. & Schwandt, D. Effective quantum dimer model for the kagome Heisenberg antiferromagnet: nearby quantum critical point and hidden degeneracy. Phys. Rev. B 81, 180402(R) (2010).
 35
Hiroi, Z. et al. Spin1/2 kagomelike lattice in volborthite Cu3V2O7(OH)2 2H2O. J. Phys. Soc. Jpn 70, 3377–3384 (2001).
 36
Matan, K. et al. Pinwheel valencebond solid and triplet excitations in the twodimensional deformed kagome lattice. Nat. Phys. 6, 865–869 (2010).
 37
White, S. R. Density matrix formulation for quantum renormalization groups. Phys. Rev. Lett. 69, 2863–2866 (1992).
Acknowledgements
We thank Keisuke Totsuka, Kenn Kubo, Karlo Penc, Hiroshi Kageyama, Yasu Takano and Peter Fulde for valuable discussions and comments. This work was supported by GrantinAid for Scientific Research (number 22014014, 20102008 and 25800204) from the Ministry of Education, Science, Sports and Culture of Japan.
Author information
Affiliations
Contributions
S.N. developed a code, carried out the DMRG simulations and analysed the data, with contributions from N.S. and C.H. C.H. brought up the project and wrote the paper, discussing with N.S. and S.N. The project was designed by all three authors and the three are equally responsible for the results.
Corresponding author
Ethics declarations
Competing interests
The authors declare no competing financial interests.
Supplementary information
Supplementary Information
Supplementary Figures S1S4 and Supplementary Notes 15 (PDF 854 kb)
Rights and permissions
About this article
Cite this article
Nishimoto, S., Shibata, N. & Hotta, C. Controlling frustrated liquids and solids with an applied field in a kagome Heisenberg antiferromagnet. Nat Commun 4, 2287 (2013). https://doi.org/10.1038/ncomms3287
Received:
Accepted:
Published:
Further reading

Effects of Dzyaloshinskii–Moriya Interactions in Volborthite: Magnetic Orders and Thermal Hall Effect
Journal of the Physical Society of Japan (2020)

Topological approach to quantum liquid ground states on geometrically frustrated Heisenberg antiferromagnets
Journal of Physics: Condensed Matter (2020)

Magnetization plateaus of spin 12 system on a 5/7 skewed ladder
Physical Review B (2020)

Enhancement of magnetization plateaus in lowdimensional spin systems
Physical Review B (2020)

FieldSelective Classical Spin Liquid and Magnetization Plateaus on Kagome Lattice
Journal of the Physical Society of Japan (2020)
Comments
By submitting a comment you agree to abide by our Terms and Community Guidelines. If you find something abusive or that does not comply with our terms or guidelines please flag it as inappropriate.